advertisement

Babar et al., International Journal of Advanced Engineering Technology E-ISSN 0976-3945 Research Paper SHEAR STRENGTH OF STEEL FIBER REINFORCED CONCRETE BEAM WITHOUT STIRRUPS V. T. Babar1, P.K. Joshi2, D.N. Shinde3 1 Address for Correspondence PG Student,2 Professor, 3Professor, Padmabhooshan Vasantraodada Patil Institute of Technology, Budhgaon, India ABSTRACT In the present dissertation work, an attempt is made to investigate shear strength and ductility of fiber reinforced concrete beams by using hooked steel fiber without stirrups and the semi-empirical equations proposed by authors in past years, are compared to find which equation holds accurate results. For this investigation, the test beam specimens of 125 mm in width, 250 mm in depth, and 1150 mm in length are cast and steel fibers are varied from 0.5 % up to 2 % volume fraction. The longitudinal steel is kept constant, while shear span-to-depth ratio (a/d) is varied in the range 1, 1.25, and 1.5. All the beam specimens are tested under two-point loading up to failure, and failure load, first crack load, and central deflection are recorded concisely and precisely. KEY WORDS: Shear Strength; beams; steel fibers; a/d ratio; concrete. 1.0 INTRODUCTION Reinforced concrete members are normally designed for the limit state of collapse in flexure rather than in shear. Shear failure, which in reality, occurs under the combined action of shearing forces and bending moments, characterized by very small deflection and lack of ductility. This failure is many times, sudden and without any warning. For this reason, shear failure is considered very undesirable and is usually avoided. The problem of shear behavior and ultimate shear strength of reinforced concrete beams was examined many years ago. Several tests were carried out and various models were developed to describe the failure behavior of reinforced concrete beams under shear forces. Many suggestions are based on the cube strength of concrete, which is still the main parameter in design principles of many countries. The research in the high strength concrete fields showed that cube strength is less important than fracture energy for the description of the material behavior of structural elements. It is well known that use of steel fibers raises the ductility of concrete and the fractured energy. This phenomenon is transferable to the shear strength of concrete. In failure modes the addition of Fibers in a suitable percentage and geometry produces a significant increase in shear strength and in some cases can also change the failure mode from shear to flexure. Also the addition of fibers can partially substitute transverse stirrups and have the same effect in terms of shear strength. They also make easy manufacture of critical portions of R.C.Structures as well as allow highly effective control of the concrete cracking process particularly in low force levels. The SFRC is a composite material made of cement, fine and coarse aggregates and discontinuous discrete steel fibers. In tension SFRC fails only after the steel fiber breaks or pulled out of the cement matrix. The composite nature of SFRC is responsible for its properties in freshly mixed and hardened state. The SFRC possess many excellent dynamic performances such as high resistance to explosion and penetration as compared to traditional concrete. The mechanical properties of SFRC are influenced by the type of fiber, aspect ratio, and volume fraction of fibers and the size of the aggregates. One of the most important properties of SFRC is its ability to transfer stresses across a cracked section which increases toughness of concrete in hardened state. Int J Adv Engg Tech/Vol. VI/Issue II/April-June,2015/15-18 Shear failure of a reinforced concrete beam occurs when the principal tensile stress within the shear span exceeds the tensile strength of concrete and a diagonal crack propagates through the beam web. This failure is usually without any warning due to the brittle nature of plain concrete behavior in tension. The addition of small discrete steel fibers into the concrete mix helps to improve the post cracking tensile strength of hardened concrete, and, hence, significantly enhances the shear strength of reinforced concrete (RC) beams. 2.0 EXPERIMENTAL PROGRAM A. Material Properties The test specimens were cast using cement, fine aggregate, coarse aggregate, water, and Hooked steel fibers. The materials, in general, confirmed to the specifications laid down in the relevant Indian Standard codes. For grading of fine and coarse aggregate, sieve analysis was carried out. Ordinary portland cement of 53-grade confirming to IS 12269:1987 was used throughout the experimental work. The maximum size of coarse aggregate used was 20 mm along with 12.5 mm of same parent rock in 60-40 % fraction. Locally available Krishna river sand was used as fine aggregate. The specific gravity of sand was 2.85 and fineness modulus was 2.7. Hooked end steel fibers of length 60 mm and diameter 0.75 mm were used throughout the experimental work. Reinforcing steel of grade Fe 500 was used as tensile reinforcement. B. Concrete Mix Design The concrete mixes were designed in accordance with the D.O.E method of concrete mix design. The concrete mix was prepared for M-25 grade of concrete. The water-cement ratio is kept at 0.45was used to enhance the workability of mix throughout experimental work. The mix proportion is given in Table I. Table I Mix Proportion C. Test Specimens Total 15 deep beams were casted. The span of the deep beam has been kept constant at 950 mm with 100 mm overhangs on either side of the supports. The a/d ratio has been kept 1,1.25,1.5. The depths of beam selected were 250 mm desire a/d ratio. All beams were rectangular in cross section with 125 mm width. Standard cubes of size 150 mm x 150 mm x Babar et al., International Journal of Advanced Engineering Technology 150 mm were cast with each mix to know the compressive strength of concrete. The details of test beams are given in Table II. E-ISSN 0976-3945 V frc (0.167 1 0.25 F ) f ' c bd where, V frc = Shear strength of FRC, = 2.5(d/a), and lf = fiber factor. F Vf df in which Vf = and fiber volume fraction, =length of fiber =diameter of fiber. IV. Mansur’s Proposed Equation [33] The equation proposed by Mansur et al[10] for shear strength of FRC is follows d V frc (0.16 f 'c 17.2 0.41F )bd a where, D. Test Procedure After 28-days curing period, the beam specimens were removed from the curing tank and both sides of the beams were white-washed to aid observations of the crack development during testing. All the beams were tested to failure under two-point loading test set-up as shown in Fig 1. The cube specimens were tested for compressive strength. Figure 1. Two point bending test set-up E. Shear Design Models Various shear strength models have been used to verify the strength of FRC deep beams in the present investigations. I. Narayanan and Darwish proposed Equation[3] By using steel fibers as shear reinforcement, Narayanan and Darwish have represented the cracking shear strength v cf as Vcf = 0.24f’spfc + 20ρ d/a + 0.5F The ultimate shear strength vuf of SFRC beams is Vuf = e [ 0.24f’spfc+ 80 ρ d/a]+ Vb where e = 1.0 when a/d> 2.8 e = 2.8d/a. when a/d< 2.8 Vb = 0.41 F = average fiber matrix interfacial bond stress, = 4.15 MPa.. II. Sharma’s proposed Equation[6] The ultimate shear strength of FRC beams has also been studied by Sharma who proposed the followingempirical equation for determining the shear strength of FRC beams. Vuf = kft(d/a)0.25 whereft= the tensile strength of concrete; and k = 1.0 ifftis obtained by direct tension test,2/3 if ftis obtained by indirect tension test, and 4/9 if ftis obtainedusing the modulus of rupture of 100-mm beams. III. Khuntia’s Proposed Equation [1] The shear strength of FRC beams is governed by the concrete contribution in the shear without stirrups and contribution of fibers. The shear strength FRC beam is given as follows, Int J Adv Engg Tech/Vol. VI/Issue II/April-June,2015/15-18 f’c =Characteristic compressive strength of concrete, = Longitudinal reinforcement ratio, and = width and effective depth of beam, a = shear span, and l f = fiber factor in which F Vf df V f = fiber volume fraction, =length of fiber and =diameter of fiber. Using equation (I) through (IV) shear strength are computed and compared with those of present investigation. 3.0 RESULTS AND DISCUSSION The results obtained from experimental investigation are tabulated in Table III. From the results obtained, the effect of various parameters on shear strength of concrete deep beam are analyzed and discussed below. A. Effect of Depth of Beam in Terms of Shear Span-to-Depth Ratio and Fiber Volume Fraction: The compressive strength, ultimate and cracking shear stress of concrete for different fiber volume fractions and shear span-to-depth ratios at 28 days of curing age are given in Table III. The variation of ultimate shear strength of deep beam with respect to fiber volume fraction for beam series I and II are given Table III. It is evident that the ultimate shear strength of deep beam increases with increase in fiber content. Fig 2 shows the effect of a/d ratio on ultimate shear strength of concrete. It is evident from the figure that the higher shear strength is developed at lower value of shear span-to-depth ratio. Ultimate shear stress at diagonal cracking, which is obtained by dividing measured failure load to the nominal cross sectional area (b x d). In deep beams, the significant portion of the shear is transmitted directly to the support by inclined strut. This mechanism is frequently referred to as arch action and the magnitude of the direct load transfer increases with decreasing a/d ratio. B. Influence on Cracking Shear Stress: Results of cracking shear stress are presented in Table III. It is concluded from Table III that cracking shear strength of deep beam increases with increase in fiber content and decreases with increase in a/d ratio. C. Influence on Cube Compressive Strength: Cube compressive strength of concrete for different fiber content is given in Table III. Cube compressive strength of concrete increases with increase in fiber content. Babar et al., International Journal of Advanced Engineering Technology E-ISSN 0976-3945 Table III Details of Test Results ultimate shear capacity. Comparison of test results E. Comparison of Test Results with Shear Design with shear design is provided in Table IV. Equation: Four design equations, namely, the Narayanan, Sharma, Khuntia and Mansur are used to estimate Table IV. Comparison of Test Results with Shear Design Equations Shear strength obtained from Sharmais lower and Narayanan is higher compared with test results, since contribution of fibers toward shear strength is not considered in above equations. Thus, Sharmaand Narayananare not applicable to compute shear strength of fiber reinforced concrete deep beams. Results obtained from Khuntia’s equation are approximately similar to test results, since contribution of fibers toward shear strength is considered. Mansur’s equation gives approximate shear strength as obtained in test for higher volume fractions. From Table IV, it is evident that, Khuntia’s equation holds good to calculate shear strength of fiber reinforced concrete deep beams. 4.0 CONCLUSION Based on the test results following conclusions can be drawn, The significant increase in compressive and split tensile strength is observed with the addition of hooked end steel fibers in plain concrete. However, this increase depends on addition of amount of fiber content. The split tensile strength went on increasing with the addition of fibers. The optimum fiber content for increase in compressive strength is 1.5%. The addition of steel fibers also decreased crack spacing and sizes, increased deformation Int J Adv Engg Tech/Vol. VI/Issue II/April-June,2015/15-18 capacity and also changed the mode of brittle failure to ductile. The ultimate shear stress is directly proportional to Percent fiber content and inversely proportional to shear span to depth ratio. Maximum percentage increase in ultimate shear stress is 60.70% for shear span-depth ratio of 1.0 and fiber content of 2.0%. The cracking shear stress is also directly proportional to fiber content and inversely proportional to shear span to depth ratio. The maximum increase in value of cracking shear stress is 54.54% compared to normal RC beams which are obtained for shear-span depth ratio of 1.0 and 2.0 % fiber content. The equation proposed by Khuntia et.al. gives fair results for shear strength of SFRC beams. This equation seems to be appropriate to estimate shear strength of normal strength concrete to high strength concrete, which shows the uniqueness of this equation. Thus, it can be proposed to include this equation in design codes of practice in case of fiber reinforced concrete beams. REFERENCES 1. Khuntia, M., Bozidar, S., and Goel, S. C., “Shear Strength of Normal and High- Strength Fiber Reinforced Concrete Beams without Stirrups”, ACI Structural Journal, Vol. 96, No. 2, July-Aug. 1999, pp. 282-290. Babar et al., International Journal of Advanced Engineering Technology 2. Kwak, Y. K., Eberhard, M. O., Kim, W. S., and Kim, J., “Shear Strength of Fiber Reinforced Concrete Beams without Stirrups”, ACI Structural Journal, Vol. 99, No. 4, July-Aug. 2002, pp. 530-538. 3. Narayanan, R., and Darwish, I. Y. S., “Use of Steel Fibers as Shear Reinforcement”, ACI Structural Journal, Vol. 84, No. 3, May-June 1987, pp. 216227. 4. Sharma, A. K., “Shear Strength of Steel Fiber Reinforced Concrete Beams”, ACI Structural Journal, Proceedings Vol. 83, No. 4, July-Aug. 1986, pp. 624628. 5. Narayanan, R., and Darwish, I. Y. S., “Fiber Concrete Deep Beams in Shear”, ACI Structural Journal, Vol. 85, No. 2, Mar.-Apr. 1988, pp. 141-149. 6. Mansur, M. A., Ong, K. C. G., and Paramsivam, P., “Shear Strength of Fibrous Concrete Beams without Stirrups”, Journal of Structural Engineering, Vol. 112, No. 9, Sept. 1986, pp. 2066-2079 7. Swamy, R. N., and Mangat, P. S., “Interfacial Bond Stress in Steel Fiber Cement Composites”, Cement and Concrete Research, Vol. 6, 1976, pp. 641-650. 8. Swamy, R. N., Jones, R. and Chiam, A. T. P., “Influence of Steel Fibers on the Shear Resistance of Lightweight Concrete T-beams”, ACI Structural Journal, Vol. 90, No. 1, Jan.-Feb. 1993, pp. 103-114. 9. Swamy, R. N., and Bahia, H. M., “Effectiveness of Steel Fibers as Shear Reinforcement”, Concrete International: Design and Construction, Vol. 7, No. 3, Mar. 1985, pp. 35-40. 10. Ashour, S. A., Hasanain, G. S., and Wafa, F. F., “Shear Behavior of High- Strength Fiber Reinforced Concrete Beams”, ACI Structural Journal, Vol. 89, No. 2, Mar.Apr. 1992, pp. 176-184. Int J Adv Engg Tech/Vol. VI/Issue II/April-June,2015/15-18 E-ISSN 0976-3945